LMucko/crystallography-open-database huggingface dataset:
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 18.85 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016855
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 18.85 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1101
_cell_length_b                   4.1101
_cell_length_c                   4.1101
_cell_formula_units_Z            4
_cell_volume                     69.432
_database_code_amcsd             0020784
_diffrn_ambient_pressure         1.885e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.369
_cod_data_source_file            inputs/fixed/downloads/05/05202.cif
_cod_data_source_block           05202
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016855
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 23.83 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016856
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 23.83 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.0824
_cell_length_b                   4.0824
_cell_length_c                   4.0824
_cell_formula_units_Z            4
_cell_volume                     68.037
_database_code_amcsd             0020785
_diffrn_ambient_pressure         2.383e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.458
_cod_data_source_file            inputs/fixed/downloads/05/05203.cif
_cod_data_source_block           05203
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016856
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 28.32 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016857
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 28.32 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.0590
_cell_length_b                   4.0590
_cell_length_c                   4.0590
_cell_formula_units_Z            4
_cell_volume                     66.874
_database_code_amcsd             0020786
_diffrn_ambient_pressure         2.832e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.536
_cod_data_source_file            inputs/fixed/downloads/05/05204.cif
_cod_data_source_block           05204
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016857
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 31.78 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016858
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 31.78 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.0410
_cell_length_b                   4.0410
_cell_length_c                   4.0410
_cell_formula_units_Z            4
_cell_volume                     65.988
_database_code_amcsd             0020787
_diffrn_ambient_pressure         3.178e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.597
_cod_data_source_file            inputs/fixed/downloads/05/05205.cif
_cod_data_source_block           05205
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016858
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 34.79 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016859
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 34.79 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.0269
_cell_length_b                   4.0269
_cell_length_c                   4.0269
_cell_formula_units_Z            4
_cell_volume                     65.300
_database_code_amcsd             0020788
_diffrn_ambient_pressure         3.479e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.645
_cod_data_source_file            inputs/fixed/downloads/05/05206.cif
_cod_data_source_block           05206
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016859
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 37.59 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016860
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 37.59 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.0148
_cell_length_b                   4.0148
_cell_length_c                   4.0148
_cell_formula_units_Z            4
_cell_volume                     64.713
_database_code_amcsd             0020789
_diffrn_ambient_pressure         3.759e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.687
_cod_data_source_file            inputs/fixed/downloads/05/05207.cif
_cod_data_source_block           05207
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016860
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 40.01 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016861
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 40.01 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.0044
_cell_length_b                   4.0044
_cell_length_c                   4.0044
_cell_formula_units_Z            4
_cell_volume                     64.211
_database_code_amcsd             0020790
_diffrn_ambient_pressure         4.001e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.724
_cod_data_source_file            inputs/fixed/downloads/05/05208.cif
_cod_data_source_block           05208
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016861
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 44.23 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016862
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 44.23 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.9877
_cell_length_b                   3.9877
_cell_length_c                   3.9877
_cell_formula_units_Z            4
_cell_volume                     63.411
_database_code_amcsd             0020791
_diffrn_ambient_pressure         4.423e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.783
_cod_data_source_file            inputs/fixed/downloads/05/05209.cif
_cod_data_source_block           05209
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016862
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 48.08 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016863
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 48.08 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.9717
_cell_length_b                   3.9717
_cell_length_c                   3.9717
_cell_formula_units_Z            4
_cell_volume                     62.651
_database_code_amcsd             0020792
_diffrn_ambient_pressure         4.808e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.841
_cod_data_source_file            inputs/fixed/downloads/05/05210.cif
_cod_data_source_block           05210
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016863
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 52.35 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016864
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 52.35 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.9525
_cell_length_b                   3.9525
_cell_length_c                   3.9525
_cell_formula_units_Z            4
_cell_volume                     61.747
_database_code_amcsd             0020793
_diffrn_ambient_pressure         5.235e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.912
_cod_data_source_file            inputs/fixed/downloads/05/05211.cif
_cod_data_source_block           05211
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016864
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 55.09 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016865
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 300 K, P = 55.09 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.9364
_cell_length_b                   3.9364
_cell_length_c                   3.9364
_cell_formula_units_Z            4
_cell_volume                     60.995
_database_code_amcsd             0020794
_diffrn_ambient_pressure         5.509e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    4.973
_cod_data_source_file            inputs/fixed/downloads/05/05212.cif
_cod_data_source_block           05212
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016865
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 700 K, P = 10.94 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016866
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 700 K, P = 10.94 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1782
_cell_length_b                   4.1782
_cell_length_c                   4.1782
_cell_formula_units_Z            4
_cell_volume                     72.940
_database_code_amcsd             0020795
_diffrn_ambient_pressure         1.094e+07
_diffrn_ambient_temperature      700
_exptl_crystal_density_diffrn    4.159
_cod_data_source_file            inputs/fixed/downloads/05/05213.cif
_cod_data_source_block           05213
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016866
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 700 K, P = 15.12 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016867
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 700 K, P = 15.12 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1450
_cell_length_b                   4.1450
_cell_length_c                   4.1450
_cell_formula_units_Z            4
_cell_volume                     71.215
_database_code_amcsd             0020796
_diffrn_ambient_pressure         1.512e+07
_diffrn_ambient_temperature      700
_exptl_crystal_density_diffrn    4.259
_cod_data_source_file            inputs/fixed/downloads/05/05214.cif
_cod_data_source_block           05214
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016867
Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O ferropericlase up to 58 GPa at 300, 700, and 1100 K Note: (Mg0.75,Fe0.25)O, T = 700 K, P = 20.51 GPa
Matsui, M.; Ito, E.; Yamazaki, D.; Yoshino, T.; Guo, X.; Shan, S.; Higo, Y.; Funakoshi, F. I.; American Mineralogist 97 (2012) 176–183; doi:

data_9016868
_publ_section_title
;
 Static compression of (Mg0.83,Fe0.17)O and (Mg0.75,Fe0.25)O
 ferropericlase up to 58 GPa at 300, 700, and 1100 K
 Note: (Mg0.75,Fe0.25)O, T = 700 K, P = 20.51 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              176
_journal_page_last               183
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Fe0.17 Mg0.83 O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1158
_cell_length_b                   4.1158
_cell_length_c                   4.1158
_cell_formula_units_Z            4
_cell_volume                     69.721
_database_code_amcsd             0020797
_diffrn_ambient_pressure         2.051e+07
_diffrn_ambient_temperature      700
_exptl_crystal_density_diffrn    4.351
_cod_data_source_file            inputs/fixed/downloads/05/05215.cif
_cod_data_source_block           05215
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(Mg.83 Fe.17) O'
_cod_database_code               9016868